Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

Materials Transactions, Vol. 54, No. 4 (2013) pp. 540 to 543 © 2013 The Japan Institute of Metals and Materials Effect of High Pressure Heat Treatment on Microstructure and Thermal Expansion Coefﬁcients of CuAl Alloy Ma Yu-quan Mechanical and Electrical Engineering College, Hebei Normal University of Science and Technology, Qinhuangdao 066004, China With different high pressure heat treatments on CuAl alloy, the effects on microstructure and thermal expansion coefﬁcients of CuAl alloy are studied in the paper by optical microscopy, scanning electron microscopy, transmission electron microscopy and expansion instrument etc. The experimental results show that after heat treatment, the structure of CuAl alloy was reﬁned obviously and the compactness increased. The grain reﬁnement effect increases at ﬁrst and then decreases when pressure is increased. When the pressure is 3 GPa, the most obvious is the thinning grain effect. In addition, the high pressure heat treatment can increase CuAl alloy thermal coefﬁcient of expansion, when the CuAl alloy is treated by 3 GPa pressure and is at 596.37°C. Thermal expansion coefﬁcient is the biggest, 3.1187 © 10¹5°C¹1, than that of the same temperature cast state samples increase 99.34%. [doi:10.2320/matertrans.M2012358] (Received October 26, 2012; Accepted January 25, 2013; Published March 25, 2013) Keywords: copperaluminum alloy, high pressure heat treatment, microstructure, thermal expansion coefﬁcient 1. Introduction CuAl alloy has been widely used in shipping, machinery, aviation and other related ﬁelds due to its high strength, corrosion resistance, excellent hot and cold processing performance. However, the coarse grains of this material restrict its further application.1) It is known that high pressure can promote the nucleation, but reduce the atomic diffusion coefﬁcient and thus restrain the grain growth.2,3) Therefore, the researches on the improvements of microstructure and properties of metal materials by means of high pressure heat treatment attracted considerable research interest.4,5) High pressure treatment has been found to be effective in improving the microstructure and mechanical properties of Cu alloys.68) However, studies on the effect of high press treatment on the thermal expansion property of Cu alloys have not been reported yet. Furthermore, the service condition for metal parts often involves the combination of thermal-dynamic coupling ﬁled, and thus it is necessary to carry out study on the effect of high pressure heat treatment on the microstructure and thermal expansion of CuAl alloy. The results reported in this paper could provide basic reference for future application of high pressure heat treatment. 2. Experiment The tested material was cast CuAl alloy whose chemical composition (mass fraction, %) is 84.67%Cu, 10.64%Al, 2.65%Fe, 1.58%Mn, 0.46% others. The samples were sealed in a graphite sleeve, and the sleeve has been embedded into the pyrophyllite mould which serves as the pressure transmitting medium. Consequently, the mould was placed into the high pressure cell of CS-IB type six-anvil high-pressure equipment as shown in Fig. 1. High pressure heat treatment involves three values: 1, 3 and 6 GPa. The samples were held at 750°C under pressure for 10 min and subsequently cooled to room temperature by cutting off the power supply with the holding pressure unchanged. Finally, the pressure was taken off. The samples before and after high pressure treatment Pressure head Samples Fig. 1 Schematic map of pressure applying on sample. were shaped into the size of º6 mm © 15 mm by electronic spark cutting, and polished with 1200# sandpaper. The thermal expansion coefﬁcient of sample in the temperature range of 25650°C were measured using a DIL402C thermal expansion instrument (using Al2O3 as reference and the precision is 3%) with a heating rate of 5°C/min under protecting of argon atmosphere. The coefﬁcient ¡ = ¦L/ (L·¦T), where ¡, L, ¦L and ¦T stands for linear expansion coefﬁcient, sample length, linear expansion of the sample and the measured temperature range, respectively. To study the phase transformation of the AlCu alloy during the temperature range of 25650°C, the thermal analyses were performed on a STA449C differential scanning calorimeter (DSC) for the samples (heated to 700°C with a heating rate of 5°C/min) before and after high pressure heat treatment. The microstructure of the samples was characterized by Axiovert 200MAT optical microscope, HATACHI S-3400N scanning electron microscope (SEM-BSE) and a JEOL-2010 transmission electron microscope (TEM). 3. Results and Discussion 3.1 Microstructure Figure 2 shows the microstructure of CuAl alloy before and after high pressure treatment. It can be seen that the microstructure of as-cast CuAl alloy was coarse. The ¡ Effect of High Pressure Heat Treatment on Microstructure and Thermal Expansion Coefﬁcients of CuAl Alloy (b) (a) 100µm 100µm (c) (d) 100µm 100µm Fig. 2 Microstructure of CuAl alloy [(a) As-cast; (b) 1 GPa; (c) 3 GPa; (d) 6 GPa]. (b) (a) 0.2µm 0.2µm Fig. 3 541 TEM images of CuAl alloy before and after high pressure treatment. [(a) As-cast; (b) 3 GPa]. (b) (a) 10µm 10µm Fig. 4 SEM-BSE images of CuAl alloy [(a) As-cast; (b) 3 GPa]. phase exists in strip pattern. After high pressure heat treatment with 16 GPa, reﬁne granular ¡ phase begin to show up and the microstructure is reﬁned signiﬁcantly. Note is the thinning effects are the most obvious when the pressure is 3 GPa. TEM observation (Fig. 3) shows that the dislocation density in CuAl alloy organizations increases after pressure process. Figure 4 is CuAl alloy SEM backscatter images before and after high pressure. As can be seen, there are more microscopic holes in the less compact as-cast CuAl alloy matrix. There is a signiﬁcant reduce of the number of microscopic holes and holes size in the matrix after high pressure heat treatment, and compact level of the matrix increase. Solid phase transformation involves nucleation and growth process of new phase which is controlled by atoms diffusion. Based on the diffusion theory, the grain size of the newly formed phase in CuAl alloy (d) can be described by following equation9) pﬃﬃﬃﬃﬃﬃ d ¼ Dt ð1Þ M. Yu-quan where is constant, D is atomic diffusion coefﬁcient, and t is diffusion time. Under high pressure, the atomic diffusion coefﬁcient (D) can be expressed as follows10) D ¼ D0 epV =RT ð2Þ where D0 is constant, P is pressure, R is gas constant, T is temperature, "V* is activation volume. The following equation may be expressed from eqs. (1) and (2): PV 1 ln d ¼ þ ln t þ ¼ 2 2RT 1.2 Heat flow, W/mW.mg-1 542 1.0 As-Cast 0.8 0.6 1GPa 0.4 0.0 100 200 Due to "V* > 0, it can be seen from eq. (3), under the same conditions, the pressure can reduce the size of the new phase grain. High degree of internal strain was introduced in the high pressure heat treated CuAl alloy, and the density of dislocation was increased by the consequently lattice distortion, providing more place that is available for the nucleation of newly formed phase and thus increasing the nucleation rate. However, the reverse effect of high pressure on the nuclear of newly formed phase begins to dominate when the pressure is higher than certain value, in which condition the atomic diffusion is prohibited. Therefore, it is reasonable to expect that there is one high pressure that can balance the increase of nucleation rate and the decrease of atomic diffusion. The resulting nucleation and growth of new phase could be promoted mostly. In this experiment, this pressure value is 3 GPa. Under this high pressure heat treatment, the nucleation rate is highest and microstructure is ﬁnest, also, the microscopic holes in the CuAl alloy matrix is closed and improve material compactness is improved by high pressure process. 3.2 DSC curves Figure 5 shows DSC curves of CuAl alloy before and after high pressure treatment at the constant heating rate of 5°C/min. One endothermic peak at 569.11572.34°C is observed on DSC curve for each heat treatment condition. Combined with Ref. 11), this endothermic peak results from the solid-state phase transformation: ¡ (Cu) + £2 (Al4Cu9) ¼ ¢ (AlCu3). 3.3 Thermal expansion coefﬁcients Figure 6 shows the relationship between the thermal expansion coefﬁcients of CuAl alloy and temperature before and after high pressure heat treatment. It can be seen that thermal expansion coefﬁcient of as-cast CuAl alloy increases with temperature from 25 to 650°C, but the changing trend is mild. When heat treated under high pressure, there is no change of the relationship between the thermal expansion coefﬁcients and temperature, but in a more rapid rate. When the temperature increase to 570°C, the thermal expansion coefﬁcients become greater increase with temperature increasing. There is a high peak for thermal 400 500 600 700 DSC curves of CuAl alloy at different states. −1 Thermal expansion coefficients × , α /10−5.°C ð4Þ 300 Temperature, T/°C Fig. 5 1 ln D0 : 2 6GP 0.2 ð3Þ where ¼ ¼ ln þ 3GPa 3.5 3GPa 3.0 6GPa 2.5 2.0 1GPa 1.5 As-cast 1.0 0.5 0 100 200 300 400 500 600 700 Temperature, T/°C Fig. 6 Relationship curves between the thermal expansion coefﬁcients of CuAl alloy and temperature. Table 1 The maximum thermal expansion coefﬁcients and its corresponding temperatures of CuAl alloy after different high pressure treatment. Pressure/GPa 1 3 6 Temperatures/°C 631.11 596.37 649.02 Thermal expansion coefﬁcients/© 10¹5°C¹1 2.6950 3.1187 0.28888 expansion coefﬁcient of CuAl alloy at temperature of 631.11 and 596.37°C after heat treatment at 1 and 3 GPa, respectively. Figure 5 also reveals that there is nearly no difference of thermal expansion coefﬁcient between different high pressure when the temperature is below around 382°C. Above this temperature, the thermal expansion coefﬁcient of sample after 3 GPa high pressure treatment is higher than that of sample treated under 1 and 6 GPa, and the difference peaks at the temperature where the highest thermal coefﬁcient arrives. The maximum thermal expansion coefﬁcients and its corresponding temperatures for each high pressure heat treatment have been tabulated in Table 1. Note that the thermal expansion coefﬁcient the sample after high pressure treatment is remarkably higher than that of the as-cast sample. After 3 GPa treatment, the highest value of the thermal expansion coefﬁcient arrives at 596.37°C with a value of 3.1187 © 10¹5°C¹1, which is about 99.34% higher than that value of the as-cast CuAl alloy at the same temperature. Effect of High Pressure Heat Treatment on Microstructure and Thermal Expansion Coefﬁcients of CuAl Alloy Since the thermal expansion of the alloy is considered to be resulted by the increase of inter-atomic distance and the void in the material can be considered as a rigid phase with zero expansion coefﬁcient12) which shows no expansion when heated. Therefore, the voids can offset the expansion of matrix, resulting the increase of compactness of material, reduce of porosity, and ﬁnally the increase of the thermal expansion coefﬁcient. High pressure treatment can also increase the compactness of CuAl alloy and decrease the residual porosity, and therefore can increase the thermal expansion coefﬁcient. In principle, high pressure would lead to a higher compactness and lower porosity level, and thus a high thermal expansion rate. However, Fig. 5 shows the thermal expansion coefﬁcient of CuAl alloy does not increases with the pressure in proportion, indicating that the thermal expansion coefﬁcient is also related to the microstructure of materials (including morphology, size, content and distribution of phase).13) Figure 5 also reveals that the maximum thermal expansion coefﬁcient happens when the applied high pressure is 3 GPa. As for the reasons why the thermal expansion coefﬁcient of samples after heat treatment under 3 GPa is higher than that of sample after other high pressure condition, and the appearance of the peak value at ¡-T curve, they need further investigation. 4. Conclusions (1) High pressure treatment can reﬁne the grain of CuAl alloy, and the most optimizing effect happens at 3 GPa in the studied press range of 1 to 6 GPa. (2) High pressure treatment can obviously increase the thermal expansion coefﬁcient of alloy in the temperature range of 25650°C, but the thermal expansion 543 coefﬁcient doesn’t increase as the pressure increases linearly. (3) Thermal expansion coefﬁcient of CuAl alloy after 3 GPa treatment reaches its maximum value at 596.37°C with a value of 3.1187 © 10¹5°C¹1, which is 99.34% higher than that of as-cast CuAl alloy at the same temperature. REFERENCES 1) G. Li, J. H. Liu, W. K. Wang and R. P. Liu: Chin. Phys. B 19 (2010) 096202. 2) Zh. X. Wang, J. B. Lu and Y. J. Xi: Mater. Sci. Eng. A 499 (2009) 192 194. 3) Z. X. Wang, F. Y. Li and M. X. Pan: J. Alloy. Compd. 388 (2005) 262 265. 4) H. W. Wang, D. D. Zhu, Ch. M. Zou and Z. J. Wei: Rare Metal Mater. Eng. 41 (2012) 4244. 5) Zh. L. Wang, T. Zhang, L. Li, Y. B. Zhou, H. W. Wang and Z. J. Wei: The Chin. J. Nonfer. Metal. 22 (2012) 10061012. 6) Y. X, Y. F. Li, F. F. Liu, J. H. Liu and R. J. Zhang: J. Mater. Sci. Eng. A 2 (2012) 8283. 7) L. L. Wu, L. Liu, J. H. Liu and R. J. Zhang: Mater. Trans. 53 (2012) 504507. 8) H. Y. Wang, J. H. Liu, G. R. Peng and W. K. Wang: Chin. Phys. B 19 (2010) 096203. 9) D. Porter and K. Easterling: Phase Transformation in Metals and Alloys, (Van Nostrand Reinhold Company, New York, 1981) pp. 263 284. 10) K. N. Ishihara, M. Maeda and P. H. Shingu: Acta Metall. 33 (1985) 21132117. 11) Zh. T. Wang: Cu Alloys and It’s Working Handbook, (Central South University Press, Changsha, 2002) p. 28. 12) F. L. Yang and D. Q. Yi: J. Mech. Eng. 45 (2009) 253257 (in Chinese). 13) B. G. Kim, S. L. Dong and Su. D. Park: Mater. Chem. Phys. 72 (2001) 4247.

Document related concepts

Hyperthermia wikipedia, lookup

Thermal conduction wikipedia, lookup

Thermoregulation wikipedia, lookup

Thermal comfort wikipedia, lookup

R-value (insulation) wikipedia, lookup

Thermal conductivity wikipedia, lookup

Passive solar building design wikipedia, lookup

Solar air conditioning wikipedia, lookup